Pré-visualização | Página 11 de 31
of the grain size. The grain size distribution of kaolin, feldspar and quartz can overlap, showing kaolin the most fine grain size, quartz with the coarser grain size and feldspar in between. In case of such mixtures, the raw materials have to be separated from each other. In case you succeed to separate the grain mixture at about 60 µm, you will get a kaolin and feldspar mixture as well as a feldspar and quartz powder mixture. 68 Fig. 2.6.1: Grain distribution of kaolin, feldspar and quartz . Fig. 2.6.2 shows schematically the selective classing of the ternary mixture kaolin, feldspar and quartz powder which can be very often found in nature. The mixture is suspended and first separated at 100-200µm. Now we have a mixture of kaolin and feldspar at the left side and at the right side a mixture of feldspar and quartz. For the separation of the kaolin- feldspar mixture we sieve at 20-40 µm. The coarse fraction contains feldspar; the fine fraction on this sieve is kaolin. In practice, the mixture usually passes through several stages of separation. Feldspar and quartz are separated at 2-4 mm and later again at 200 µm. The coarse fraction is quartz sand. The fine fraction is again separated into fine quartz powder and a fraction of feldspar. 69 Fig. 2.6.2: Separation of three products via selective separation/ grinding . Fig. 2.6.3 shows schematically a complete preparation of kaolin. The raw materials are charged to the grinding mills and larger stones with diameters within centimetre area are separated from the residual material. The screenings are homogenised with water by adding dispersants in order to charge the particles’ surface and reduce the water content during processing. Coarse fractions are separated from the fine ones in log washers and washing mills. 70 Fig. 2.6.3: Kaolin preparation, flowchart of a general wet process . The fine content is further processed in hydro-cyclones at different stages. Separation grain size is about 20-40 µm. Fig. 2.6.4 shows how a hydro cyclone works. This hydro cyclone is loaded in radial direction with a suspension. Two flow cycles are formed due to the special geometry: the inner flow which in the underflow takes up the coarse fraction and the external spiral which discharges the fine fraction at the top. The cyclone’s geometry effects separation within a certain grain size area. The more exact grain separation is required, the more hydro cyclone series have to be operated in succession. 71 Fig. 2.6.4: Functional scheme of a hydrocyclone . 72 Fig. 2.6.5: Flowchart of a Kaolin preparation plant . Fig. 2.6.5 demonstrates schematically the multi-stage cyclone separation in a kaolin preparation plant. The fines sediment in large slurry tanks, a procedure which we know from sewage works. After sedimentation and filtration the material is dried in drying aggregates and stored in silos or transported in bags to the customers. Videoclip: Raw material preparation „The material is transported on conveyors from the mine to a preparation hall. The first log washer separates the coarse grains from the fine ones. The coarse material sediments on the bottom and is transported by bowls to the next step of separation. The fine suspension is separated at the other side of the log washer and transported to these cyclones. Before, the mixture is cleaned in sieves and the fines are separated from the coarsest grains. In the background you see the multi-staged cyclone steps. The coarse material is carried on to bunkers and later-on in another video we will pick up the material to get it crushed. But first it has to undergo several sieve levels and log washers where the coarse fraction is again separated from the finer one.” 73 Fig. 2.6.6: Hydro-separator (classifier and concentrator) . English china clay lovering, Pochin&Co.Ltd., Cornwall. After leaving the hydro cyclones the water has to be separated from the solids. This is made in large slurry tanks (Fig. 2.6.6). The coarse fraction mostly consists of a feldspar-quartz- mixture. Feldspar and quartz can be separated in electrostatic drum cobbers. For this, the feldspar and quartz surfaces have to be charged. Chemical reagents are added attaching to the surface. The charging process of feldspar and quartz surface is varyingly strong (Fig. 2.6.7). 74 Fig. 2.6.7: Electric charging of quartz and feldspar versus temperature . The distinct electrostatic surface charges are used to separate the material, for example, in a drum cobber. An electric field is set up on a turning roll. Highly charged material will be higher deflected, while less strong charged material will be less deflected. And in this way with these drum cobbers quartz and feldspar can be separated. In praxis this separation is made in fully automated plants (Fig. 2.6.8). First a sand mixture of feldspar and quartz runs into a preheated drum. The surfaces of feldspar and quartz are charged varyingly strong by a treatment in HF and the raw materials are separated in multi-staged drum cobbers. 75 Fig. 2.6.8: Flowchart of electrostatic separation of quartz and feldspar . Flotation is another possibility for material separation. As already discussed, long-chain molecules can be docked onto charged surfaces. Docking behaviour varies because the materials’ crystal structure is different. This means, for instance, that particles with a higher addition of organic additives in a water barrel can be dragged-out to the top. As for quartz, for example, relatively few long-chain molecules attach to the surface, but much more with regard to orthoclase (Fig. 2.6.9). When a quartz-feldspar mixture is dispersed in water, the feldspar particles float towards the top and can be taken off, while the quartz particles sediment to the bottom. 76 Fig. 2.6.9: Flotation behaviour of quartz and orthoclase as a function of the pH in HF-acidic suspension with Dodecylammonium chloride (500g/t) . Upward current classification is another possibility for material separation (Fig. 2.6.10). The material to be classified is led to a case filled with a liquid and with water streaming in from the bottom. A soft water movement from the bottom to the top appears. The coarse particles sediment downward and are collected in the first bunker. The fine particles stay longer in the suspension phase and sediment in the rear tanks. Prior to further processing the suspensions respectively sediments have to be separated into solids and liquids. 77 Fig. 2.6.10: Working principle of multi-chamber upward classifiers (schematic) . This can be done in different appliances. Planar filters (Fig. 2.6.11), for example, consist of a filtration level and an extruding screw which extrudes the material sedimenting on this filtration level. The filtrate can be removed from the bottom. Separation of powder and water can also be made in so-called rotary dryers where the material is given into a turning drum with a slight down-grade (Fig. 2.6.12). The material rotates at a turning drum motion to the left, while in the opposite direction hot air is applied to the material which has to be dried. Fig. 2.6.11: Cross-section of a planar filter for quartz-sand dehydration . 78 Fig. 2.6.12: Rotary dryer . Another variation is the water jet dryer (Fig. 2.6.13). The compound being charged can first be led to a crushing appliance and is then injected into a hot gas path.